Template-free synthesis of mesoporous
manganese oxides with catalytic activity in the
oxygen evolution reaction
Suoyuan Lian,‡aMichelle P. Browne,‡aCarlota Dom´ınguez,aSerban N. Stamatin,a Hugo Nolan,aGeorg S. Duesberg,aMichael E. G. Lyons, aEmiliano Fondab and Paula E. Colavita *a
Porous manganese carbonate was obtained viasolvothermal synthesis using ethanol and urea. The manganese carbonate was subsequently used as a precursor to synthesise mesoporous manganese oxides via thermal treatments at three various temperatures. X-ray diﬀraction and Extended X-ray Absorption Fine Structure (EXAFS) results shows that g-MnO2 is synthesised at 380 and 450C while Mn2O3is produced at the annealing temperature of 575C. X-ray absorption spectra show thatg-MnO2 converts completely to Mn2O3 after annealing over the 450–575 C range. The oxides obtained at 380 C and 450 C possess extremely high speciﬁc surface area, which is of interest for catalytic applications. The oxides were investigated as electrocatalysts for the oxygen evolution reaction; the oxide prepared at the lowest annealing temperature was found to be the optimum catalyst with an overpotential of 42710 mV at a current density of 10 mA cm2, normalised by the geometric area. The improved catalytic activity was related to the presence of defect-rich and highly porous manganese dioxide at the lowest annealing temperature.
It is estimated that the world's current fossil fuel reserve will be depleted within the next century, therefore alternative routes to the production of energy are urgently needed and further inte-gration of renewable sources into the energy economy will be necessary over the next decades.1,2 Alkaline water electrolysis,
when coupled with renewable sources, can provide a clean and environmentally friendly path for the production of H2, an
alternative fuel.3,4 Fuel cells that use H
2 and O2 can produce
electric power on demand to supply the national grid or to power car transport, with the major advantage to this energy route that emissions are limited to water.5,6Unfortunately, most
of the H2 currently used in fuel cells is generated by steam
reforming of fossil fuels, while the percentage that comes directly from water electrolysis only accounts for 4%.7,8Since
the discovery of water electrolysis by van Troostwijk and Dei-man, the technology of water electrolysis has indeed been
commercially developed, but is economically limited by the rare and expensive materials needed as electrocatalysts.9,10
Water electrolysis results in the formation of O2at the anode, via the oxygen evolution reaction (OER), and of H2 at the
cathode. Even though the main goal for energy applications is to generate H2 at the cathode, the majority of research eﬀorts
concentrate on the anodic reaction. The OER is the rate deter-mining step of water electrolysis which also makes it the most energy demanding electrode process; therefore, a reduction in the OER overpotential can translate into greater eﬃciency in hydrogen production.6 To date, RuO
2is regarded as the most
active OER catalyst in alkaline media as this oxide catalyses water oxidation at the lowest known overpotentials at a current density of 10 mA cm2.11,12However, its commercial application
is limited owing to its high cost and low abundance.13
Transition metal oxides (TMOs), from the rst row of the periodic table, in particular Mn, Fe, Co and Ni oxides, are viable candidates to replace IrO2 and RuO2 as OER catalysts.14,15
Currently in literature, a vast number of reports on water oxida-tion focus on applicaoxida-tions of nickel, cobalt and iron oxides as electrocatalysts; however, there has been a recent increased interest in investigating manganese oxides as catalysts for the OER.2,16–29 Some of the reported OER activities of manganese
oxides in literature are extremely encouraging.11,30–33Suibet al.
studied the OER capabilities of three phases of MnO2,a,bandg,
on a carbon support that were fabricated through three similar hydrothermal routes. The overpotential at 10 mA cm2for thea,
aSchool of Chemistry, CRANN and AMBER Research Centres, Trinity College Dublin,
College Green, Dublin 2, Ireland. E-mail: email@example.com
bSynchrotron SOLEIL L'Orme de Merisiers, St Aubin BP48, 91192 Gif sur Yvette Cedex,
†Electronic supplementary information (ESI) available: Further characterisation data including an image of MnOxpowders, Raman, XAS, XRD and LSVs. See DOI: 10.1039/c7se00086c
Cite this:Sustainable Energy Fuels, 2017,1, 780
Received 10th February 2017 Accepted 11th April 2017
Energy & Fuels
Published on 12 April 2017. Downloaded on 09/02/2018 12:34:47.
View Article Online
bandgphases were 0.49, 0.60 and 0.74 V, respectively.30These
results indicate that small changes in the synthetic method alter the resulting phase and the OER activity. Commercial MnO, Mn3O4, Mn2O3 and MnO2 powder samples, made into an ink
dispersion, were deposited onto a glassy carbon substrate and tested as OER catalysts by Jaramilloet al.34The overpotentials of
0.51, 0.43, 0.53 and 0.5 V were reached to obtain a current density of 10 mA cm2for the MnO, Mn3O4, Mn2O3and MnO2,
respec-tively. Interestingly, Fiechteret al.fabricated Mn3O4and Mn2O3
by an electrodeposition/thermal process.35 This study showed
that the Mn2O3was a superior OER catalyst when compared to
Mn3O4, which contradicted the previous report by Jaramillo et al.34,35Additionally the MnO
2materials produced by Jaramillo et al.and Suibet al.also exhibited varying overpotential values at 10 mA cm2. Therefore, the specic fabrication process used to synthesise the Mn oxide clearly plays a critical role in deter-mining the activity of the material for the OER.
The physical structure of the OER catalysts, such as shape or surface area, strongly aﬀects their performance.19,36–38 The
surface area of a material has been previously linked to an increase in the OER catalytic activity of metal oxides due to the potential increased density of active sites.39 Solvothermal
synthesis can be used to fabricate porous materials,40 most
notably using soor hard templates;41,42however, the templates
required for the formation of porous products must be etched post synthesis and this removal stage is time consuming and adds to the complexity of the process. A solution to this consists of using precursors that decompose into gaseous products so that gas bubbles template pore formation during the synthesis. Lian et al., has previously used urea as a precipitant for the formation of metal hydroxides and aer annealing, a porous structure remains.43Precipitants such as urea or NH
routinely used under hydrothermal conditions however in this study urea will be used under solvothermal conditions.43–46
Synthesis of Mn oxides for OER applicationsviasolvothermal methods is relatively underexplored compared to electrochemical and thermal methods.19,28,31,35,47In this work, porous MnCO
synthesised by a template free solvothermal-urea method; urea was used as the precipitant and ethanol as the solvent under solvothermal conditions. Solvothermal conditions were preferred over hydrothermal conditions as ethanol results in higher pres-sure in a closed reactor compared to water at the same temper-ature, which was expected to promote porosity in the carbonate material. The resulting MnCO3was used as a precursor for the
subsequent preparation of Mn oxidesviathermal decomposition at diﬀerent temperatures. The materials were characterised by a variety of techniques to determine composition, morphology, and surface area. Voltammetry experiments in alkaline media show that the synthesised oxides are active in the OER; trends in onset potential are interpreted and discussed in relation to the structural and morphological properties.
Chemicals and materials
Manganese acetate ($99% metal basis), sodium hydroxide pellets ($98%, reagent-grade), urea and Naon-117
(reagent-grade) were purchased from Sigma and used without further purication; ethanol (reagent grade, >99%) was purchased from the TCD solvent facility.
In a typical synthesis, 0.30 g Mn(CH3COO)2$6H2O, 0.35 g urea
and 11 mL ethanol were mixed together directly in an 18 mL Teon-lined stainless steel autoclave (Yuhua Instrument CO., LTD). The autoclave was sealed and placed inside the oven and heated at 140C, 160C or 180C for 24 h. Aer the reaction time, the autoclave was allowed to cool to room temperature under natural convection. Samples were centrifuged and washed alternately in ethanol and Millipore water, 4 times, and
nally dried at 50C for 12 h. Annealing of the resulting MnCO3
was carried out at 380, 450 and 575C for 4 h in a tube furnace in air and the resulting MnOxwere denoted as Mn-380, Mn-450,
Emission Scanning Electron Microscope (SEM) was carried out using a Karl Zeiss Ultra Field Emission Scanning Electron Microscope (SEM) at 5 kV accelerating voltage and 5 mm working distance using a Secondary Electron (SE) detector. Transmission Electron Microscopy (TEM) was performed using a JEOL JEM-2100 TEM at an accelerating voltage of 200 kV; samples were mounted on holey carbon/copper grids (S147, Agar Scientic). Powder X-ray diﬀraction (XRD) patterns were collected in a Bruker D2 Phaser with a Cu Kasource (l¼1.5418
A). Specic surface area measurements were carried out on a Quantachrome Autosorb iQ, running nitrogen physisorption measurements at 77 K. Thermogravimetric analysis (TGA) was conducted on a Pyris 1 Thermogravimetric Analyzer (Perki-nElmer) with a 5 C min1 temperature ramp, using air as carrier gas. Raman spectroscopy measurements were performed using a Witec alpha 300R confocal Raman microscope using a 1800 line mm1grating and a 532 nm diode laser at an
inci-dent power of <10 mW and a spot size of 300 nm.
ray absorption near edge structure (XANES) and Extended X-ray Absorption Fine Structure (EXAFS) measurements were undertaken at the SAMBA beamline at SOLEIL synchrotron, France.48Pellets were fabricated using cellulose and 6 wt% of the
relevant Mn material then mounted in a holder for analysis; all pellets were measured in transmittance mode at the Mn K-edge. Reference samples (purchased from Sigma) of MnO (man-ganosite), Mn3O4 (hausmannite), a-Mn2O3 and b-MnO2 were
recorded in addition to synthesised samples for the analysis of edge positions. All samples were calibrated using a Mn foil during the experiments. Data analysis was performed using Athena and Artemis soware packages;49calculation of scattering paths was
carried out using FEFF v.8.4 and self-consistent potentials.50
EXAFS data was extracted as described by Newvilleet al.51 with
aRbkg¼1. The Fourier Transform (FT) was performed betweenk¼
3 and 10.5A˚1with a Hanning apodization window with sills of amplitude dk¼1. The EXAFS signal was weighted byk3andtted inr-space between 1 and 4A; both real and imaginary parts were˚
tted according to the procedure described by Newville.52
All electrochemical experiments were carried out in a standard three-electrode cell using a high performance digital potentio-stat (CH model 1760 D Bi-potentiopotentio-stat). A graphitic carbon rod was used as counter electrode. The potential was recorded using an Hg/HgO reference electrode (CH instruments, #152); all potentials are reported vs. the reversible hydrogen electrode based on the following equation:ERHE¼EHgO/Hg+ 0.059(pH) +
0.098 V. The working electrode (WE) consisted of ITO glass (7 ohm per sq, Xin Yan Technology Ltd.) on which the relevant solvothermal material was deposited from an ink dispersion. The inks were prepared as follows: 10 mg of manganese-containing powders were mixed with 8mL of Naon solution and 400mL ethanol, followed by sonication for 1 h. 20mL of the dispersion was then dropped onto the ITO glass over a 77 mm2surface area dened by masking tape resulting in a 1 mg
cm2loading for all samples; current densities were calculated
based on the geometric area dened by the mask. Linear sweep voltammetry (LSV) was conducted in 1 M NaOH solution at a scan rate of 5 mV s1 in the anodic direction. All measure-ments were conducted at a constant temperature of 25C, using a thermal bath with the temperature maintained by a thermo-stat. All plotted data are presented in iR compensated form; the iR compensation was calculated from a built-in iR compensa-tion module in the CH-instrument soware.
Results and discussion
The solvothermal synthesis of manganese carbonate (MnCO3)
from the acetate in the presence of urea was carried out at 140, 160 and 180C in order to determine at what temperature the pure carbonate is obtained. The colors of the powders obtained at the three temperatures, Fig. S1,†are diﬀerent, whereby the solids formed at 140, 160 and 180C were brown, light brown and white, respectively. Aer synthesis, X-ray diﬀraction (XRD) was performed on all of the samples, Fig. 1a. XRD analysis reveals that solids prepared at 140C display reections from both MnCO3 and Mn3O4 (COD: 9007691 and COD: 9001302).
Aer increasing the temperature to 160C, the Mn3O4 re
ec-tions are less visible, indicating that the Mn3O4 decomposes
and the MnCO3becomes the major component. At 180C, the
results show that the powder is completely composed of MnCO3. Brunauer Emmett Teller (BET) analysis of nitrogen
adsorption isotherms for samples prepared at 180C yielded a specic surface area of 100 m2g1; thus indicating that the synthesis in the presence of urea results in a porous solid.
Thermogravimetric analysis (TGA) was also performed on the three synthesised MnCO3 to investigate phase changes
during the thermal treatment in air to determine which powder would be the best precursor for producing metal oxides, Fig. 1b. The loss of mass in the temperature region of 0–220C can be attributed to the loss of approximately 5% of water for all the MnCO3powders. At 220C, the MnCO3is known to decompose
to form MnO2 as discussed by Zhu et al.53 For the sample
prepared at 180C, the weight loss, aer accounting for the loss of water, is approximately 31%, which is in agreement with
a transition from MnCO3to Mn2O3.54The samples prepared at
160C and 140C have a lower weight loss of 24% and 23%, which suggests the co-existence of lower Mn oxide species aer thermal treatment, likely associated with the presence of Mn3O4
identied in the XRD of the starting sample (Fig. 1a). The signicant weight loss resulting from decomposition of the sample prepared at 180C indicates that this is the precursor compound that results in the greatest gas evolution, thus sug-gesting potential for high porosity upon thermal treatment. Since high specic surface area is a desirable property for applications in catalysis, the MnCO3synthesised at 180C was
henceforth chosen as the precursor for the formation of the Mn oxide catalysts for OER.
Characterisation of oxides obtained from MnCO3precursor
The MnCO3was further annealed in air at 380, 450 and 575C
to produce diﬀerent oxide materials, denoted Mn-380, Mn-450 and Mn-575, for testing in the OER. The resulting oxides and the MnCO3precursor were characterised in terms of porosity,
morphology and structure using a combination of nitrogen adsorption analysis, scanning and transmission electron microscopy (SEM, TEM), XRD and X-ray absorption spectros-copy (XAS).
Nitrogen adsorption/desorption isotherms were analysed to determine specic surface area and pore size distribution of the MnCO3 precursor and of the oxides obtained aer thermal Fig. 1 XRD (a) and TGA (b) of solid samples prepared from the sol-vothermal reaction of manganese acetate in the presence of urea at three diﬀerent temperatures. Diﬀraction peaks associated to Mn3O4 (o) and to MnCO3(c) are labeled in (a).
treatment in air, Fig. 2 and Table 1. Fig. 2a, shows that all samples display characteristic type-IV adsorption isotherms.55
The specic surface areas calculated using the BET method are reported in Table 1; results indicate that the carbonate precursor has an initially high porosity of 100 m2g1which is
high compared to a previously reported commercial MnCO3
sample with a value of 11.3 m2g1and to some of the recently
reported porous MnCO3.53,56 Aer thermal treatment, the
materials formed remain highly porous aer annealing treat-ments at 380 and 450C, while the surface area collapses aer annealing at 575C. The BET surface areas of the Mn-380 and the Mn-450 materials are signicantly higher than those typi-cally reported in literature for Mn oxides from thermal decomposition of MnCO3.57,58The pore size distribution of all
samples obtainedviaBarrett–Joyner–Halenda (BJH) analysis of desorption branches can be observed in Fig. 2b. For the as-prepared MnCO3, the pore size is predominately in the range
of 1.5–2.5 nm, while aer annealing at 380, 450 or 575 C, a maximum in the pore size distribution develops in the range 3–10 nm; this indicates that gas evolution aer thermal treat-ment of MnCO3leads to the opening of pores in the mesopore
range. The use of ethanol as the solvent was crucial for the development of a porous structure in MnCO3, as shown by the
synthesis of MnCO3using hydrothermal conditions. Fig. 2a and
b show the adsorption/desorption isotherms and BJH pore
distribution, respectively, of the hydrothermal precursor. Almost no hysteresis loop is observed in Fig. 2a suggesting that no porous structure forms during the hydrothermal process of the same materials, and the BET surface area was 90% lower than that obtained under solvothermal conditions.
All of the materials aer the annealing treatment were comprised of sheets or particles which group together to form spherical structures, Fig. 2c–e. Aer the preparation of the dispersionviasonication the spherical structures are disrupted resulting in solid particles that could be deposited onto solid surfaces, as shown in Fig. 2f–h. There was no apparent variation observed in the morphology of the Mn-380 and Mn-450 samples whereas particles in the Mn-575 appear smaller when compared to the lower annealing temperatures.
Fig. 2 (a) Nitrogen adsorption/desorption isotherms and (b) BJH pore size distribution diagram of MnCO3, Mn-380, Mn-450 and Mn-575 (c) SEM image of as-prepared Mn-380 (d) SEM image of as-prepared Mn-450 (e) SEM image of as-prepared Mn-575 and (f) SEM image of Mn-380 as aﬁlm, (g) SEM image of Mn-450 and (h) SEM image of Mn-575.
Table 1 Speciﬁc surface area of precursor MnCO3and of samples after thermal annealing in air at 380, 450 and 575C
BET area (m2g1)
Changes in particle morphology were further investigatedvia
TEM; Fig. 3a–d show images of the MnCO3precursor and the
Mn-380, Mn-450 and Mn-575 powders. Before any heat treat-ment to the MnCO3, the solid particles display a nanosheet-like
morphology, Fig. 3a, with the size of these MnCO3nanosheets
in the range 100–200 nm. Aer thermal treatment at 380 and 450 C, a sheet-like morphology is still present the MnCO3
precursor particles. Aer thermal treatment at 575C a signi -cant change in morphology is observed, whereby particles appear to be denser.
The XRD patterns of the precursor MnCO3 and of the
compounds obtained aer thermal treatment at 380, 450 and 575 C are shown in Fig. 4a. Upon increasing annealing temperature it can be observed that the XRD pattern is dramatically altered from the MnCO3starting material. For the
MnCO3, all peaks can be indexed to a standard MnCO3(COD:
9007691) as previously discussed. The sample treated at the lowest temperature of 380C exhibits broad peaks that are in agreement with those reported for electrolytic manganese dioxides (EMD), Fig. 4b.61EMD is proposed to be composed of
both3-MnO2andg-MnO2, howeverg-MnO2is the predominant
phase.61The reections at 23.0, 37.0, 42.1, 55.2and 66.3are
in agreement with the EMD structure studied by Simonet al.61
while an additional broad peak at 31.4can be attributed to the starting material, MnCO3. Raman analysis of the Mn-380
sample (see ESI†) also indicates that a phase of MnO2 is
present, Fig. S2;†the intense peak at 661 cm1can be attributed to3-MnO2in agreement with results reported by Linet al.60,61
Aer thermal treatment at 450 C, the XRD pattern displays similar reections to those of Mn-380, while additional peaks consistent with the presence of Mn2O3are also evident at 33.0,
55.2 and 65.8, Fig. 4c.19 Aer treatment at 575C the XRD
pattern displays narrow peaks, Fig. 4d, that can all be indexed to standard Mn2O3(COD: 9007520), thus indicating the complete
conversion of the material to pure Mn2O3 oxide phase. The
Raman spectrum for Mn-575 also conrms a change in the oxide structure, with peaks in agreement with those observed for Mn2O3by Julienet al.62
The presence of broad peaks and mixed phases in XRD patterns indicates that materials obtained from the thermal decomposition of MnCO3in air possess low crystallinity and are
structurally disordered. XAS was therefore used to characterise MnCO3and MnOxpowders. Normalised absorption spectra at
the Mn K-edge for MnCO3, Mn-380, Mn-450 and Mn-575
samples are shown in Fig. 5a. The absorption edge energy of Mn-380 and Mn-450 is higher than that of Mn-575, thus indi-cating that Mn-centres in MnOxpowders synthesised at 380 and
450C have a higher average oxidation state than in the MnOx
powder annealed at 575C.63A comparison with the precursor
MnCO3sample also shows that in all cases the oxidation state is
higher than that in the carbonate precursor. The normalised X-ray absorption near edge (XANES) spectra of 380 and Mn-450 samples are indistinguishable thus indicating that their structure is similar, in agreement with XRD results. The XANES of Mn-575 samples was found to match that of Mn2O3, as shown
in Fig. 5b, also conrming the XRD assignments. The Mn-380 sample could not be tted through a combination of any of the reference samples tested and its structure was determined
via further analysis of the extended X-ray absorption ne structure (EXAFS) spectrum as discussed below.
To conrm the presence of3-MnO2and/org-MnO2in
Mn-380 suggested by the XRD pattern, the EXAFS spectrum was
tted inRspace, Fig. 5c; thet presented includes only single scattering contributions up to 4A and was obtained by˚ xingS02
at 0.8. The positions and amplitudes of the main peaks in the bestt match the coordination number (N) and distances (R) of the Mn–O(1), Mn–Mn(1), Mn–O(2) and Mn–Mn(2) coordination shells ofg-MnO2. The scattering path parametersNandR
ob-tained for the bestt of Mn-380 can be observed in Table 2 and are in excellent agreement with those reported by Godartet al.
for g-MnO2;64 the mean-square displacements are relatively
large and indicate signicant disorder in the oxide structure. Fits which included coordination shells characteristic of 3 -MnO2resulted in a signicant reduction in the goodness oft
(see ESI, Fig. S3†). In summary, XAS results show that Mn-380 and Mn-450 samples consist of predominantly g-MnO2,
whereas Mn-575 samples mainly consist of Mn2O3.
OER performance of manganese oxides
The linear sweep voltammetry (LSV) curves for the precursor MnCO3and the various Mn oxides can be observed in Fig. 6; LSV
curves plotted as a function of overpotential are reported in the ESI.† The three MnOx samples show enhanced OER activity
when compared with the MnCO3 as all three oxide materials
yield higher anodic currents when compared to the MnCO3. In
current literature, the activities of OER materials are ranked by how low the overpotential value is at a current density of 10 mA cm2. The reporting of the overpotential values at a current
density of 10 mA cm2is related to the energy produced for the utilisation of a water electrolyser linked to a 10% eﬃcient solar cell and is the most commongure of merit when comparing OER catalysts.11,18,19,31
The Mn-380 exhibits the highest activity for OER and the overpotential (h) at a current density of 10 mA cm2is 427
Fig. 3 TEM images of (a) MnCO3, (b) 380 (c) 450 and (d) Mn-575. Scale bar for all images is shown in (d).
10 mV. The overpotentials at the same current density for the Mn-450 and Mn-575 materials are 470 10 mV and 570 20 mV, respectively. The MnCO3starting material proves to be
very inactive for the OER as it only reaches a current density of approximately 0.72 mA cm2 at the overpotential of 570 mV. The relative order of activity is the same also when the current density is normalized by the BET area of each material (see Fig. S5†). This result indicates that the annealing step is a crit-ical step in this study. The overpotentials were found to be constant over three cycles for all materials; however stability over prolonged cycling was limited by physical spalling during OER due to low adhesion between the ITO support and the oxide. This suggests that mechanical stability of the supported particles must be optimised for future device applications, as previously noted for other OER catalysts.65
The improved performance of the Mn-380 is likely related to the specic oxide phase and/or the increased surface area of this material. The structure of the sample is consistent with that observed for highly disordered MnO2phases, based
on both XRD and XAS. The Mn–O(1) distance is typical of Mn(IV)/Mn(III) oxides,17 while the Mn–Mn(1) distance
indi-cates the presence of edge-sharing MnO6 octahedra, oen
associated with catalytically active MnOx.17,26,29 High
struc-tural disorder, as evidenced by XRD and XAS in this sample, is also associated with activity in the OER.26,29It is interesting to
note that a Mn–Mn(1) 2.91 A distance is somewhat longer˚ than that observed for di-m-oxo bridged Mn(IV) centres, this
being typically 2.86A.˚27,29This is suggestive of the presence of
a fraction of Mn(IV)–(m-O)2–Mn(III) contributions27that cannot
be resolved but that are consistent with the high values of Debye Waller factors obtained in our ts. It is a current hypothesis that disordered Mn oxides with valences above (III)
and below (IV) are active in OER.27–29,66 A plot of the edge
position against the Mn-oxidation state for reference samples used in our XAS experiments can be used to approximate the oxidation state of Mn-centres via a linear interpolation, as previously shown in the literature.27,59This approach shows
that Mn-380 has an oxidation state intermediate between (III)
and (IV) (see Fig. S7†), again supporting the presence of
defects and vacancies that result in mixed Mn-valence and contribute to OER activity. The presence of mixed Mn(III)/
Mn(IV) centres in disordered and layered MnO2 oxides is
known to result in slow, long-term transformations (over months/years) that result from stress releaseviamigration of Mn(III) centres and cation rearrangement.67 Accordingly, we
have observed similar slow transformations in the most active Mn-380, as shown by the slow appearance of additional reections in the XRD pattern upon prolongued ageing (see Fig. S8†), which are accompanied by a reduction of activity compared to freshly prepared samples. This is not observed in the case of the least active materials, thus indicating that high OER activity is associated to a defect-rich metastable oxide phase in agreement with other oxides with reported high activity in the OER.68Finally, the Mn-380 also exhibits
the largest surface area which is also consistent with this being the most active of the oxides examined.
Fig. 4 (a) XRD pattern of MnCO3, Mn-380, Mn-450 and Mn-575; (b) Mn-380 and (c) Mn-450 compared tog-MnO2and3-MnO2patterns from literature;59,60(d) Mn-575 compared to COD reference for Mn
The Mn-450 shows a very slight increase in the amount of Mn2O3, based on its XRD pattern, when compared to the
Mn-380 and a slight decrease in the BET surface area. Samples treated in air at 575C are completely converted to Mn2O3, and
the surface area also decreases drastically. From the LSV curves, a reduction in the OER performance can be observed for the
Mn-575, therefore this decrease may be linked to the decrease in surface area and the presence of Mn2O3which is proposed to be
less active than MnO2phases in the OER.69
When comparing with literature values, the Mn-380 has an improved OER activity compared to the most active manganese oxide catalysts prepared by Suib et al.30 The hydrothermally
produced a-MnO2 oxide exhibited BET surface area values of
112 m2g1and an overpotential value at 10 mA cm2of 490 mV.
It is evident that the surface area of Mn-380 in this study and the MnO2 prepared by Suib et al. are similar. Hence, the
over-potential decrease of 60 mV for the Mn-380 in this study is likely attributable to the improved performance of the specic oxide phase,i.e.g-MnO2vs.a-MnO2. The Mn-380 also has improved
OER capabilities when compared to other manganese oxides produced by wet chemistry methods in literature.26,35,40 This
might be attributable to the manganese carbonate synthesised solvothermally in this study, which oﬀers a robust mesoporous structure as a precursor platform for the further synthesis of the OER active Mn-380 material. Even aer annealing at 380C, the mesoporous structure can still be retained aer the MnO2phase
Pure manganese carbonate (MnCO3) was obtained through
a template-free solvothermal synthesis at 180C. The manga-nese carbonate was used as a precursor to fabricate mangamanga-nese oxidesviathermal treatment in air at diﬀerent temperatures. XRD, Raman and XAS results show that a highly disordered MnO2phase is synthesised at temperatures of 380C and 450C
while Mn2O3 is produced at 575 C. Interestingly, the EXAFS
analysis of the sample obtained at 380C shows that this oxide is largely composed ofg-MnO2. BET analysis indicates that the
highest surface area is retained for the Mn oxide made at 380 C, with pore sizes in the mesoporous range, while it decreases with treatment at higher temperatures.
All of the oxides were tested as catalysts for the OER and the sample prepared at 380 C was found to exhibit the lowest
Fig. 5 (a) Mn K-edge absorption thresholds for the MnCO3, Mn-380, Mn-480 and Mn-575 (b) XANES for the Mn-575 with the Mn2O3 reference and (c) EXAFSﬁt (continuous lines) for the neighbors of the central Mn atom obtained using theg-MnO2structure for the Mn-380 sample (dotted lines); the modulus and imaginary parts of the Fourier Transform (FT) function are reported in black and red, respectively.
Table 2 Scattering paths used for the bestﬁt of the EXAFS spectrum of Mn-380 samples
Path R(A)˚ N s2(˚A2)
Mn–O(1) 1.92(1) 6 0.008(2)
Mn–Mn(1) 2.91(2) 2 0.009(3)
Mn–O(2) 3.25(3) 2 0.04(1)
Mn–Mn(2) 3.50(3) 8 0.016(4)
Fig. 6 Linear sweep voltammetry curves of solvothermally prepared MnCO3, Mn-380, Mn-450 and Mn-575; data was collected in 1 M NaOH at 5 mV s1. All electrodes were fabricated by the same method with aﬁnal loading of 1 mg cm2of the relevant material drop cast onto the substrate.
overpotential at a current density of 10 mA cm2 of 427 10 mV. This performance when compared to that of oxides obtained at higher temperatures is likely due to both the high specic surface area of the material and the specic oxide phase (g-MnO2) that results from the thermal process. In conclusion,
these results indicate that solvothermal synthesis of MnCO3is
a viable route for the facile synthesis of electroactive meso-porous manganese dioxide. Interestingly, the material exhibits catalytic activity in the OER that is similar to or better than other MnOxcatalysts currently in literature thus opening the
possi-bility of a new family of low-cost OER catalysts for water splitting.
The manuscript was written through contributions of M. P. B, P. E. C and S. L. The concept and execution of the synthesis was carried out by S. L. XRD was carried out by S. L and M. P. B. Microscopy was carried out by S. L. XANES and EXAFS measurements were performed by M. P. B, C. D, E. F and P. E. C. Linear combinationtting and EXAFS analysis was done by M. P. B and E. F. The electrochemistry was done by S. L and M. P. B. Raman analysis was performed by H. N. BET and BJH was done by S. N. S. All authors have given approval to thenal version of the manuscript.
This publication has emanated from research conducted with thenancial support of the Irish Research CouncilviaGrant No. GOIPD/2014/68 and of Science Foundation Ireland (SFI) grant No. 13/CDA/2213; MPB also acknowledges support from SFI Grant No. 12/RC/2302. We acknowledge SOLEIL for provision of synchrotron radiation facilities through Grant No. 20150740.
ict of interest
The authors declare no competingnancial interests.
The authors are grateful to the SAMBA staﬀfor assistance with XAS measurements and to the staﬀin the AML, CRANN for help with the SEM and TEM analysis, particularly D. Daly and E. McCarthy. We would also like to thank Dr B. Twamley for help with the XRD analysis. The authors would like to thank the Schmitt group in the School of Chemistry in TCD for access to their BET instrumentation. Finally, the authors are grateful to Prof. Yang Liu from the Institute of Functional Nano and So Materials (FUNSOM) for kindly providing the autoclaves.
1 S. Shaee and E. Topal,Energy Policy, 2009,37, 181–189. 2 M. Gong and H. Dai,Nano Res., 2015,8, 23–39.
3 S. Cho, Y. B. Woo, B. S. Kim and J. Kim,Biomass Bioenergy, 2016,87, 144–155.
4 Y. Cheng and S. P. Jiang,Prog. Nat. Sci., 2015,25, 545–553. 5 M. Carmo, D. L. Fritz, J. Merge and D. Stolten,Int. J. Hydrogen
Energy, 2013,38, 4901–4934.
6 M. E. G. Lyons, R. L. Doyle, D. Fernandez, I. J. Godwin, M. P. Browne and A. Rovetta,Electrochem. Commun., 2014,
7 M. Balat,Int. J. Hydrogen Energy, 2008,33, 4013–4029. 8 S. E. Hosseini and M. A. Wahid,Renewable Sustainable Energy
Rev., 2016,57, 850–866.
9 R. de Levie,J. Electroanal. Chem., 1999,476, 92–93. 10 S. Trasatti,J. Electroanal. Chem., 1999,476, 90–91.
11 C. C. L. McCrory, S. Jung, I. M. Ferrer, S. M. Chatman, J. C. Peters and T. F. Jaramillo, J. Am. Chem. Soc., 2015,
12 W. Hu, Y. Q. Wang, X. H. Hu, Y. Q. Zhou and S. L. Chen,J. Mater. Chem., 2012,22, 6010–6016.
13 C. Jin, F. L. Lu, X. C. Cao, Z. R. Yang and R. Z. Yang,J. Mater. Chem. A, 2013,1, 12170–12177.
14 B. M. Hunter, H. B. Gray and A. M. M¨uller,Chem. Rev., 2016,
15 E. Fabbri, A. Habereder, K. Waltar, R. Kotz and T. J. Schmidt,
Catal. Sci. Technol., 2014,4, 3800–3821.
16 M. P. Browne, J. M. Vasconcelos, J. Coelho, M. O'Brien, A. Rovetta, E. K. McCarthy, H. Nolan, G. Duesberg, V. Nicolosi, P. E. Colavita and M. Lyons,Sustainable Energy & Fuels, 2017,1, 207–216.
17 A. Indra, P. W. Menezes, I. Zaharieva, E. Baktash, J. Pfrommer, M. Schwarze, H. Dau and M. Driess, Angew. Chem., 2013,52, 13206–13210.
18 M. P. Browne, S. Staﬀord, M. O'Brien, H. Nolan, N. C. Berner, G. S. Duesberg, P. E. Colavita and M. E. G. Lyons,J. Mater. Chem. A, 2016,4, 11397–11407.
19 M. P. Browne, H. Nolan, G. S. Duesberg, P. E. Colavita and M. E. G. Lyons,ACS Catal., 2016,6, 2408–2415.
20 J. R. Swierk, S. Klaus, L. Trotochaud, A. T. Bell and T. D. Tilley,J. Phys. Chem. C, 2015,119, 19022–19029. 21 H. Ali-L¨oytty, M. W. Louie, M. R. Singh, L. Li, H. G. Sanchez
Casalongue, H. Ogasawara, E. J. Crumlin, Z. Liu, A. T. Bell, A. Nilsson and D. Friebel, J. Phys. Chem. C, 2016, 120, 2247–2253.
22 S. Klaus, Y. Cai, M. W. Louie, L. Trotochaud and A. T. Bell,J. Phys. Chem. C, 2015,119, 7243–7254.
23 J. Wang, W. Cui, Q. Liu, Z. Xing, A. M. Asiri and X. Sun,Adv. Mater., 2016,28, 215–230.
24 E. L. Tae, J. Song, A. R. Lee, C. H. Kim, S. Yoon, I. C. Hwang, M. G. Kim and K. B. Yoon,ACS Catal., 2015,5, 5525–5529. 25 N.-I. Kim, Y. J. Sa, S.-H. Cho, I. So, K. Kwon, S. H. Joo and
J.-Y. Park,J. Electrochem. Soc., 2016,163, F3020–F3028. 26 A. Indra, P. W. Menezes and M. Driess,ChemSusChem, 2015,
27 A. Bergmann, I. Zaharieva, H. Dau and P. Strasser,Energy Environ. Sci., 2013,6, 2745–2755.
28 Y. Gorlin, B. Lassalle-Kaiser, J. D. Benck, S. Gul, S. M. Webb, V. K. Yachandra, J. Yano and T. F. Jaramillo,J. Am. Chem. Soc., 2013,135, 8525–8534.
29 I. Zaharieva, P. Chernev, M. Risch, K. Klingan, M. Kohlhoﬀ, A. Fischer and H. Dau,Energy Environ. Sci., 2012,5, 7081–7089.
30 Y. Meng, W. Song, H. Huang, Z. Ren, S.-Y. Chen and S. L. Suib,J. Am. Chem. Soc., 2014,136, 11452–11464. 31 Y. Gorlin and T. F. Jaramillo,J. Electrochem. Soc., 2012,159,
32 L. C. Seitz, T. J. P. Hersbach, D. Nordlund and T. F. Jaramillo,
J. Phys. Chem. Lett., 2015,6, 4178–4183.
33 M. Browne, R. J. Cullen, R. L. Doyle, P. E. Colavita and M. E. G. Lyons,ECS Trans., 2013,53, 59–77.
34 S. Jung, C. C. L. McCrory, I. M. Ferrer, J. C. Peters and T. F. Jaramillo,J. Mater. Chem. A, 2016,4, 3068–3076. 35 A. Ramirez, P. Hillebrand, D. Stellmach, M. M. May,
P. Bogdanoﬀand S. Fiechter, J. Phys. Chem. C, 2014,118, 14073–14081.
36 K. C. Neyerlin, G. Bugosh, R. Forgie, Z. C. Liu and P. Strasser,
J. Electrochem. Soc., 2009,156, B363–B369.
37 L. Xu, Q. Q. Jiang, Z. H. Xiao, X. Y. Li, J. Huo, S. Y. Wang and L. M. Dai,Angew. Chem., Int. Ed., 2016,55, 5277–5281. 38 A. R. Zeradjanin, A. A. Topalov, Q. Van Overmeere,
S. Cherevko, X. Chen, E. Ventosa, W. Schuhmann and K. J. J. Mayrhofer,RSC Adv., 2014,4, 9579–9587.
39 X. Z. Cui, Z. L. Hua, L. S. Chen, X. H. Zhang, H. R. Chen and J. L. Shi,ChemSusChem, 2016,9, 1010–1019.
40 C. H. Kuo, I. M. Mosa, A. S. Poyraz, S. Biswas, A. M. E-Sawy, W. Q. Song, Z. Luo, S. Y. Chen, J. F. Rusling, J. He and S. L. Suib,ACS Catal., 2015,5, 1693–1699.
41 B. Solsona, T. Garcia, R. Sanchis, M. D. Soriano, M. Moreno, E. Rodriguez-Castellon, S. Agouram, A. Dejoz and J. M. L. Nieto,Chem. Eng. J., 2016,290, 273–281.
42 R. D. Zhang, P. X. Li, N. Liu, W. R. Yue and B. H. Chen,J. Mater. Chem. A, 2014,2, 17329–17340.
43 S. Y. Lian, E. Wang, Z. H. Kang, Y. P. Bai, L. Gao, M. Jiang, C. W. Hu and L. Xu,Solid State Commun., 2004,129, 485–490. 44 M. Pudukudy, Z. Yaakob and R. Rajendran, Mater. Lett.,
45 X. L. Wu, M. H. Cao, H. Y. Lu, X. Y. He and C. W. Hu,J. Nanosci. Nanotechnol., 2006,6, 2123–2128.
46 X. C. Duan, J. B. Lian, J. M. Ma, T. Kim and W. Z. Zheng,
Cryst. Growth Des., 2010,10, 4449–4455.
47 J. L. Fern´andez, M. R. Gennero De Chialvo and A. C. Chialvo,
J. Appl. Electrochem., 2002,32, 513–520.
48 V. Briois, E. Fonda, S. Belin, L. Barthe, C. La Fontaine, F. Langlois, M. Ribbens and F. Villain, UVX 2010-10e Colloque sur les Sources Coh´erentes et Incoh´erentes UV, VUV et X, Applications et D´eveloppements R´ecents, 2011, pp. 41–47. 49 B. Ravel and M. Newville,J. Synchrotron Radiat., 2005,12,
50 A. L. Ankudinov, B. Ravel, J. J. Rehr and S. D. Conradson,
Phys. Rev. B: Condens. Matter Mater. Phys., 1998, 58, 7565– 7576.
51 M. Newville, P. L¯ivin¸ˇs, Y. Yacoby, J. J. Rehr and E. A. Stern,
Phys. Rev. B: Condens. Matter Mater. Phys., 1993,47, 14126– 14131.
52 M. Newville,J. Synchrotron Radiat., 2001,8, 322–324. 53 C. Zhu, G. Saito and T. Akiyama,J. Mater. Chem. A, 2013,1,
54 L. Biernacki and S. Pokrzywnicki,J. Therm. Anal. Calorim., 1999,55, 227–232.
55 K. S. W. Sing,Pure Appl. Chem., 1985,57, 603.
56 W. Kang, D. Y. W. Yu, W. Li, Z. Zhang, X. Yang, T.-W. Ng, R. Zou, Y. Tang, W. Zhang and C.-S. Lee,Nanoscale, 2015,
57 S. H. Lee, Y. Kwon, S. Park, M. Cho and Y. Lee,J. Mater. Sci., 2015,50, 5952–5959.
58 X. Tan, Y. Wan, Y. Huang, C. He, Z. Zhang, Z. He, L. Hu, J. Zeng and D. Shu,J. Hazard. Mater., 2017,321, 162–172. 59 S. J. A. Figueroa, F. G. Requejo, E. J. Lede, L. Lamaita,
M. A. Peluso and J. E. Sambeth, Catal. Today, 2005, 107– 108, 849–855.
60 M. Lin, B. Chen, X. Wu, J. Qian, L. Fei, W. Lu, L. W. H. Chan and J. Yuan,Nanoscale, 2016,8, 1854–1860.
61 D. E. Simon, R. W. Morton and J. J. Gislason, Adv. X-Ray Anal., 2004,47, 267.
62 C. M. Julien, M. Massot and C. Poinsignon, Spectrochim. Acta, Part A, 2004,60, 689–700.
63 A. Manceau, M. A. Marcus and S. Grangeon, Am. Mineral., 2012,97, 816.
64 C. Godart, M. Latroche, C. Freticny and C. Levy-Clement,
Phys. Status Solidi A, 1992,132, 253–268.
65 M. E. G. Lyons, R. L. Doyle, M. P. Browne, I. J. Godwin and A. A. S. Rovetta,Curr. Top. Electrochem., 2017,1, 40–45. 66 I. Zaharieva, D. Gonzalez-Flores, B. Asfari, C. Pasquini,
M. R. Mohammadi, K. Klingan, I. Zizak, S. Loos, P. Chernev and H. Dau,Energy Environ. Sci., 2016,9, 2433– 2443.
67 S. Grangeon, B. Lanson and M. Lanson, Acta Crystallogr., Sect. B: Struct. Sci., 2014,70, 828–838.
68 J. A. Bau, E. J. Luber and J. M. Buriak, ACS Appl. Mater. Interfaces, 2015,7, 19755–19763.
69 H.-Y. Su, Y. Gorlin, I. C. Man, F. Calle-Vallejo, J. K. Norskov, T. F. Jaramillo and J. Rossmeisl,Phys. Chem. Chem. Phys., 2012,14, 14010–14022.